Highly reversible capacity at the surface of a lithium-rich manganese oxide: a model study using an epitaxial film system †

Epitaxial films of Li 2 MnO 3 were synthesized using pulsed laser deposition. A 12.6 nm film exhibited a high discharge capacity of over 300 mA h g (cid:2) 1 following its fiftieth cycle and better stability than 29.8 and 47.8 nm films. The surfaces of such films are intrinsically active at the electrochemical interface. Lithium-rich manganese oxide (Li 2 MnO 3 ) is one of the most promis-ing candidates for a lithium battery cathode material, due to its high charge–discharge capacity of over 250 mA h g (cid:2) 1 . 1–4 Although Li 2 MnO 3 has been reported to be intrinsically inactive with regard to lithium deintercalation as a result of the high valence state of Mn 4+ , 5 nanosized Li 2 MnO 3 is activated upon initial charging cycle by the release of oxygen from the lattice to the electrolyte. 6 The resulting oxygen-deficient phase is transformed to a phase that exhibits reversible lithium (de)intercalation. However, the use of Li 2 MnO 3 presents a significant challenge due to the significant reduction in discharge capacity and discharge voltage upon cycling. issue, and obtaining 3 the of the electrochemical is initiated at the electrode/electrolyte radiation. Elemental Li and Mn ratios were determined from ICP-MS (Agilent Technologies, 7500cs) analyses of samples dissolved in aqua regia diluted with ultrapure water at 373 K for 30 min. XANES measurements were performed in the fluorescence mode using a germanium single-element solid-state detector installed at SPring-8 BL14B2 and data were collected at an oblique incidence angle of 4 1 . Pre-edge back-ground and post-edge normalizations of spectra to unity were performed using the ATHENA software package. 13 The oxidation

This journal is © The Royal Society of Chemistry 2015 states of Mn ions in the films were from Mn 3s HAXPES spectra acquired at SPring-8 BL46XU using a hemispherical electron energy analyzer (SCIENTA, R-4000) with an incident photon energy level of approximately 7940 eV and a photoelectron take-off angle of 801.The binding energy was calibrated according to the Au 4f 7/2 core level spectrum.Neutron reflectometry was performed using a time-of-flight reflectometer (SOFIA) installed at J-PARC BL16. 14,15The Parratt32 program, which applies Parratt's method, 16 was used for reflectivity data analysis. 17harge-discharge characteristics were examined using 2032type coin cells assembled in an argon-filled glovebox.
The counter/reference electrodes were lithium metal and the electrolyte was 1 mol dm À3 LiPF 6 an ethylene carbonate-diethyl carbonate mixture (3 : 7, v/v).All cell tests were conducted at 298 K.No significant changes in the crystal structure or the composition were observed when varying the film thicknesses (Fig. S3 and S4 in ESI †).
The ratio of lithium to manganese atoms in the Li 2 MnO 3 film was estimated by ICP-MS analysis to be Li : Mn = 1.85(7) : 1.The origin of the compositional deviation was investigated by XANES, HAXPES and neutron reflectometry analyses.Fig. 2a shows the XANES spectrum obtained from a Li 2 MnO 3 (001) film and from polycrystalline Li 2 MnO 3 powder.The XANES spectrum and the E 0 value of the film indicate that its structure and oxidation state are identical to those of polycrystalline Li 2 MnO 3 .The oxidation state of the Mn can be determined from the difference in the binding energies of the two separated Mn 3s peaks in the HAXPES spectrum. 20,21The HAXPES spectrum in Fig. 2b shows a difference in the peak positions of 4.3 eV, corresponding to Mn IV (4.4 eV).Both the XANES and HAXPES results show that tetravalent Mn is present in the film; therefore, there were no significant changes in the valence state of Mn.This result demonstrates that the film is deficient in both lithium and oxygen and thus has the composition Li 2À2x Mn(IV)O 3Àx as a result of charge compensation.
Neutron reflectometry was employed to analyse the extent of the lithium and oxygen deficiencies in the films, due to its high sensitivity for light elements. 17   (SLD) profile of a Li 2 MnO 3 (001) film.A three-layer composed of Li 2 MnO 3 /SrRuO 3 /SrTiO 3 generated the best fit to the reflectivity curve.The thickness, surface roughness and SLD values of the film were 45.1 nm, 5.4 nm and 1.97 Â 10 À4 nm À2 , respectively.The SLD is defined according to the following equation.
Here r is the SLD, M is the molecular weight, b is the overall scattering length in the unit cell and N A is Avogadro's number.The lithium and oxygen deficiencies in the film were estimated using the SLD value, together with the formula Li 2À2x Mn(IV)O 3Àx and a lattice volume of 200.9(14)Å 3 determined from neutron reflectometry, HAXPES and XRD.In this manner, the value of x was determined to be 0.05.A Li/Mn ratio of 1.90 is consistent with the results of ICP analysis (1.86 (7)).Thus, we may conclude that the films had the chemical formula Li 1.90 Mn(IV)O 2.95 .The synthesis of Li 2Àx MnO 3Ày by the chemical treatment of nanosized Li 2 MnO 3 with LiH has been reported. 22In the present study, the direct synthesis of lithium and oxygen deficient lithium-rich manganese oxide was successfully achieved using PLD.The formation of a deficient phase is expected, given the low partial pressures of lithium and oxygen and the high temperature applied during the synthesis. 23ig. 4 presents charge-discharge curves of 47.8, 29.8 and 12.6 nm thick Li 2 MnO 3 (001) films.Upon the initial charging, the voltage increased gradually from 3.8 to 4.6 V and then plateaued.A potential slope is often observed with nanosized film electrodes because of side reactions that are quite prominent due to the small amount of active material. 246][27][28] All the films exhibited reversible charge-discharge reactions upon subsequent cycling.The initial discharge capacities increased with decreasing film thickness from 47.8 nm (120 mA h g À1 ) through 29.8 nm (194 mA h g À1 ) to 12.6 nm (279 mA h g À1 ).Furthermore, the discharge capacity of the 12.6 nm thick film gradually increased with subsequent cycles to reach 318 mA h g À1 in the fiftieth cycle.The 3 V region in the discharge curves of the 12.6 nm thick film showed an increase in the capacity during the cycling, indicating a transition to another phase.The average discharge potential was 3.26 V in the first cycle and remained relatively stable at 3.24 V by the fiftieth cycle.The phase transition in the 12.6 nm thick film resulted in the increase in the discharge capacity with no significant fading of the discharging potential.The discharge capacities and cycling stability of the 12.6 nm thick film were superior to those previously reported for Li 2 MnO 3 with particle sizes of 70 nm (140 mA h g À1 in the tenth cycle) 6 and 50 nm (240 mA h g À1 in the tenth cycle).
To clarify the thickness dependence of the capacities, the reaction potentials of the active phase were investigated.The differential capacity plots during the initial ten cycles are shown as the inset in Fig. 4.After the electrochemical activation at the first charging, all films exhibited two cathodic peaks at around 3.4 V and 2.9 V and two anodic peaks at around 3.0 and 4.4 V.No significant differences in the potentials were observed depending on the film thickness, which reveals that the similar active phase was formed in the 12.6, 29.8, and 47.8 nm thick films.Hence the high capacity observed for the 12.6 nm thick film demonstrates the high electrochemical activity at the surface region of the Li 2 MnO 3 .
The transformation from pristine Li 2 MnO 3 to the active phase is followed by the extraction of lithium and oxygen at the electrode/electrolyte interface, so that oxygen ions must diffuse from the Li 2 MnO 3 bulk to the interface during the initial activation process.Considering the low diffusion coefficient of oxygen in Li 2 MnO 3 at room temperature, it is reasonable to conclude that oxygen release occurs primarily in the surface region of the electrode.An influence of the high electric field at the interface could be another driving force for the release of oxygen from the electrode surface.As a detailed activation mechanism, it has been proposed that the extraction of lithium in the transition metal layer causes migration of transition metals to the lithium layer and tetrahedral lithium formation, which causes a phase transition at the first charging. 29A first-principles study Li 2 MnO 3 has suggested that the lithium ions in the lithium layer participate in the lithium extraction at the beginning of charging, followed by the lithium removal from the transition metal layer. 30In contrast, lithium ions in the transitional layer should participate in the lithium extraction at the beginning of charging in our Li 2 MnO 3 films with the restricted reaction plane of (001). 31,32The facile formation of lithium deficiency in the transition metal layers could be related to the higher electrochemical activity of the Li 2 MnO 3 (001) film electrodes than that of polycrystalline Li 2 MnO 3 previously reported.Further investigation based on structural analyses is needed to clarify the detailed mechanism.
Previous reports have suggested various strategies to promote the initial activation.Specifically, nanosizing enlarges the contact area of the Li 2 MnO 3 particles with the electrolyte, which enhances the activation frequency, 6,33 stepwise charging could promote structural rearrangement under mild conditions, 34 leading to good reversibility of the lithium (de)intercalation into the reconstructed Li 2 MnO 3 22 and, lastly, a large number of stacking faults are formed in nanosized Li 2 MnO 3 when applying a low temperature during synthesis to reduce the particle size, implying that stacking faults lead to high electrochemical activity. 6Based on these mechanisms, pre-reduction to form a disordered arrangement prior to electrochemical cycling is accepted as an effective means of achieving the facile activation of the layered Li 2 MnO 3Àd phase. 22However, the higher capacity and better stability of the 12.6 nm thick film compared to the 47.8 and 29.8 nm thick films cannot be explained based on these factors, since these films all had the same contact area, the electrochemical tests were performed under the same conditions with no stepwise charging, and the films had similar ordering structures and lithium and oxygen deficiencies.Our results obtained using these model electrodes offer new insight into the activation process of lithium-rich layered cathodes; the surface region of the electrode is intrinsically active with regard to the electrochemically induced transformation to a high capacity phase exhibiting high electrochemical stability.In summary, epitaxial Li 2 MnO 3 (001) films were successfully synthesized on SrRuO 3 /SrTiO 3 (001) substrates using PLD.The films generated 00l and 0k0 XRD peaks showing a monoclinic lattice along the SrTiO 3 [111] and [1-10] directions.Lithium and oxygen vacancies were determined in these films, which were assigned the chemical composition Li 1.90 Mn IV O 2.95 .The 12.6 nm thick film showed higher capacity over 300 mA h g À1 and better stability compared to the 29.8 and 47.8 nm thick films.The dependence of the electrochemical properties on the film thickness demonstrates that the surface region is actively reconstructed to generate a highcapacity phase with high electrochemical stability.
This work was supported by the Research and Development Initiative for Scientific Innovation of New Generation Battery (RISING Project) of the New Energy and Industrial Technology Development Organization (NEDO; Japan).The synchrotron X-ray experiments were performed as projects approved by the Japan Synchrotron Radiation Research Institute (2013B1530 and 2013B1711), and the neutron experiments were performed as projects approved by the Japan Proton Accelerator Research Complex (2013B0166).

Fig. 1
shows the out-of-plane XRD patterns of a Li 2 MnO 3 film.The film generated diffraction peaks at 18.81, 38.11 and 81.31 along the out-of-plane [111] direction, which are attributed to the 00l diffraction peaks of Li 2 MnO 3 with the C2/m space group.The 020 and 060 diffraction peaks were observed along the in-plane [1-10] direction at 20.71 and 65.31, respectively (Fig. S1 in ESI †).The 020 peak is attributed to a superlattice structure with honeycomb Li/Mn ordering in the transition metal layer. 18No diffraction peaks of other phases were observed in the XRD patterns, confirming the single phase formation of a lithium-rich layered Li 2 MnO 3 .The rocking curve of the 020 reflection indicates six-fold symmetry at intervals of 601 (Fig. S2 in ESI †).Although the 020 reflection should have two-fold symmetry, the six-fold symmetry demonstrates that the Li 2 MnO 3 (001) film is composed of 601-rotated domains.The cell parameters are calculated to be a = 4.953(14) Å, b = 8.579(4) Å, c = 5.0095(8) Å, and b = 109.235(5)1.

Fig. 3
Fig. 3 Neutron reflectometry results for an epitaxial Li 2 MnO 3 (001) film.The insets show the fitting model and the SLD profile calculated using the fitting parameters.

Fig. 4
Fig. 4 Charge-discharge curves and differential capacity plots for Li 2 MnO 3 (001) films with thicknesses of (a) 47.8 nm, (b) 29.8 nm and (c) 12.6 nm, measured over the range from 2.0 to 4.8 V with current densities of 602.5, 103.3 and 516.5 mA g À1 , respectively.